The Area Ratio for Odd-Shaped Stencil Apertures

Joey writes:

Dear Dr. Ron,

I have a stencil aperture with an unusual shape. See Figure 1. How do I calculate the area ratio? The stencil thickness is 5 mils. The dimensions of the aperture are also in mils.

Joey,

The area ratio is simply the area of the stencil aperture opening divided by the area of the sidewalls. For common aperture geometries such as circles, squares, etc. it is easy to derive formulas. See Figure 2.

For an unusual shape like yours, it is easiest to simply calculate and divide the areas. From Figure 1, we get that area of the aperture opening as: 40*24+ the area of the two triangles. A little geometry (can you do it?) shows each triangle to have an area of 89 sq mils. So, the total area is 960 + 2*89 = 1138 sq mils. The perimeter is 40+24+16+16+28+12+16+16 = 168 mils, hence the area of the sidewalls is 168*5 = 840 sq mils. Therefore, the area ratio is 1138/840 = 1.355. Experience has shown that an area ratio of > 0.66 is needed for good solder paste transfer efficiency, so this stencil aperture will do well for transfer efficiency.

Careful thought would suggest that the triangular protrusions alone do not have a good area ratio. Calculations show their area ratios to be 0.37. So, the transfer efficiency in this part of the aperture might not be good. However, the area of the rectangle is so great, more than five times that of the triangles, as to alleviate this concern.

Dr. Ron

Does Solder Paste’s “Five Ball Rule” Remain Valid in SMT Today?

Folks,

My good friends, Phil Zarrow and Jim Hall, in their audio series “Board Talk,” were recently asked about the “Five Ball Rule”. In the comments section for this session, one listener asked if this rule, created in the 1990s, was still valid. After all, the 1990s was the era of 0603 and 0402 passives; 01005 and even 008004 passives have arrived.

First, let’s consider what a “rule” is verses a “law.” As an example of a law, consider Newton’s Laws of Motion. At everyday speeds, these laws are shown to be accurate to within our capability to measure. As we will recall from Physics 101, these laws were superseded by Einstein’s Theory of Relativity, at speeds close to those of the speed of light. However, in our everyday world, Newton’s Laws are well … laws. They are, for practical purposes, exact.

What is a “rule” then? A rule is an expression that approximately fits some empirical data or the experience of experts. Moore’s Law is actually a rule, as it is not precise. The doubling of transistor density has varied from every 18 months to every two years. That’s why I call it a rule, a very useful rule indeed!

The “Five Ball Rule” is clearly a rule. It was likely developed a generation ago by some of the first SMT pioneers. It may be backed up by experiment, but I think it was likely more a consensus of SMT industry authorities from the 1980s and 1990s.

What is the “Five Ball Rule?” It states that the solder paste’s largest solder particle diameter should be such that at least five of these particle diameters would span the width of a rectangular stencil aperture (Figure 1).

Figure 1. The Five Ball Rule

When this rule was developed, stencil apertures were much coarser than today, and the finest solder powder was a Type 3, with Type 4 on the horizon. While it is true that stencil aperture widths are much finer today, solder pastes of Type 4.5, 5, and even 6 are now in use.

The particle sizes of different “Type” solder pastes are shown in Figure 2. Note that, for Type 4 powder, 80% by weight of the particle diameters are between 20 and 38 microns. 38 microns is considered the “largest particle.” So, from Figure 2, for Type 5 powder, the “largest particle” is 25 microns. For the sake of the Five Ball Rule, the “largest particle,” for each powder type are those shown in Figure 2.

Figure 2. Solder Powder Sizes.

So, is the Five Ball Rule still valid? It would be hard to argue that it is not. Hundreds of experiments have been performed using the Five Ball Rule, combined with the aperture ratio being >1.5 for rectangular apertures or the area ratio being > 0.66 for square or circular apertures, with successful results.

StencilCoach software now includes the newer (finer) solder powder sizes to 1) tell the user the fineness of solder paste powder for the Five Ball Rule, as well as 2) help with calculating aperture or area ratio. By the way, some have suggested that, for a square or circular aperture, an “Eight Ball Rule” is more appropriate. So, StencilCoach uses the Eight Ball Rule for such apertures.

Cheers,

Dr. Ron